1 Acta of Bioengineering and Biomechanics Vol. 15, No. 1, 2013 Original paper DOI: /abb Retention force assessment in conical crowns in different material combinations JAN K. PIETRUSKI 1 *, EUGENIUSZ SAJEWICZ 2, JACEK SUDNIK 2, MAŁGORZATA D. PIETRUSKA 1,3 1 Dental Practice, Białystok, Poland. 2 Białystok University of Technology, Faculty of Mechanical Engineering, Poland. 3 Medical University of Białystok, Department of Periodontal and Oral Mucosa Diseases, Poland. The puprose of this study was to evaluate retention force of conical double crowns in two material connections: gold casting alloy/gold casting alloy and gold casting alloy/gold electroforming alloy. 12 crown pairs of both material connections with the cone angles of 2, 4 and 6 were made. Experiment of in-and-out cycles was performed using a new device which allows the retentive force to be measured in continuous way without necessity of moving the samples to another device. It has been found that the higher the retentive force values, the lower the cone angle. Dispersion of the retention value was similar in both groups, but when cone angle was 2 or 4, stability of retention force with the passage of time was higher in combinations with electroformed copings. The optimum solution was the cast alloy/cast alloy connection but only with cone angle 6. However, retentive values seem to be too low to achieve proper retention of dentures. Key words: retention force, conical crowns, gold casting alloy, gold electroforming alloy 1. Introduction Removable dentures supported by double crowns have been successfully used for years in dentistry. The crowns are usually conically shaped, or cylindrical. Conical double crowns are used both in partially dentate patients, including those with compromised dentition, and in edentulous subjects with dental implants  . They offer a safe way to combine teeth and implants in one construction . Proper functioning of this type of dentures is largely dependent on precision both in the dental surgery and laboratory, on the experience of dental technicians and clinicians and on the course of technological processes associated with denture making. Their manufacturing process, especially in the case of traditional lost-wax technique where both the primary and secondary crowns have to be hand-made and fitted, depends on technician s skills and precision and this makes sometimes the final effect difficult to predict. Ensuring proper retentive force is indispensable for normal functioning of conical crown dentures. This force should be neither too strong so as not to damage the periodontium or implant connection when the denture is taken off, nor too weak, to prevent uncontrolled loss of retention during mastication. However, above all, the retentive force should be characterized by a possibly constant value both with reference to the successive removal/insertions and long-term wear. This can be achieved only when permanent conditions of widely understood tribology effects between contact surfaces of primary and secondary crowns are maintained. This, however, is difficult to obtain in practice. In order to improve retentive force stability, novel constructions and technologies with the use of new material combinations are implemented  . Due to the advancement of prosthetic techniques used * Corresponding author: Jan K. Pietruski, Dental Practice, ul. Waszyngtona 1/34, Białystok, Poland. Tel/fax: , Received: November 30th, 2011 Accepted for publication: September 28th, 2012
2 36 J.K. PIETRUSKI et al. for the double crowns, electroforming and CAD-CAM methods can be employed, apart from the classic lostwax casting method. The use of electroforming to produce a secondary crown eliminates the handmodelling phase and fitting, as the secondary crown is electrolytically made on the primary crown. It has also been shown that the use of leucite ceramics (Empress 1) for the primary crown and the use of the electroforming method to make the secondary crown may bring promising results, both in terms of retentive force and its repeatability . The implementation of new options for conical crowns, both in terms of construction, technology or material, requires testing, with special attention paid to the value and stability of the retentive force. In earlier long-term follow up studies analyzing operational reliability of dentures made in different technologies it was found that use of electroforming in manufacturing double crown dentures gives rise to much higher percentage of mechanical failures. More complicated constructions in which electroformed copings are glued into metal framework makes the denture more susceptible to mechanical failures like copings coming unstuck, veneering material chipping or framework fractures . That is why a question arises whether use of these new technologies like electroforming is really worth taking the risk of higher failure rates. For obvious reasons, broad-scope studies can only be performed in vitro. Up to now, no standard has been designed for such studies, and many different methods and appliances have been used. One of the simpler techniques is to measure the retentive force by manual separation of denture components using a standard dynamometer . However, such measurements provide only limited data concerning retention and a long-term research is impossible to perform. Currently, a two-stage test procedure is a major technique. During the first stage, the definite number of joining and separating cycles are performed using a specially designed device and then the pair tested is fixed onto another appliance where measurements are performed to measure the retentive force , , , . This procedure shows the empirical relationship between the number of cycles and retentive force. However, a comparison of results reported by various authors reveals a fundamental inconsistency, more in the character than in the value of the changes observed. Some investigators have found a decrease in retentive force along with an increasing number of cycles, whereas others have reported a non-established character of changes, including increase , , , . One of the reasons may be that the first experimental phase is performed either in dry conditions or in the presence of artificial saliva ,  . Also measurements of retentive force during the second phase of experiments were usually conducted dry, even if a liquid environment was used in the first phase , . Moreover, process of sample removal from the testing machine and mounting it on the measuring device can cause differences in position of inner and outer crown relatively to each other. If this is so, it can have influence on reliability of measurements, because together with changing position of one of the crowns, retention force is changing, too. However, more important is that the authors cited above seem to focus rather on tendencies in the changes in retentive force and not on its stability ,  . Despite the considerable dispersion of the experimental data, Weigl and Lauer  were the ones to notice the significance of this problem for the functioning of dentures supported by conical crowns. The repeatability of retentive force is the key problem here, for it is the great variation of the retentive force values between the successive joining/separating cycles, and not the averaged force value that determines proper retention of the connection. This two-phase procedure cannot be employed for the experimental testing of retentive force stability as it does not allow step-by-step recording, being only capable of recording changes in retentive force in the respective cycle intervals. In this way, it precludes the analysis of the history that is hidden in an averaged course of changes. Since the methods used so far to test retention have major limitations, the authors made an attempt to design a device that would allow more complete analysis of changes in retentive force of conical crowns. It was accepted that the retentive force would be measured for each joining/separating cycle, and that both joining of the denture components and their separating as well as the accompanying measurement of retentive force would be performed on the same device. The potential of the device was verified experimentally, assessing the effect of the crown taper and type of the materials combination on the level and stability of retentive force. With the use of the new device an experiment was planned, the objective of which was to: 1. asses retention force values depending on geometrical parameters of conical crowns; 2. asses retention force values depending on technology and material used to make primary and secondary crown in combinations: cast gold/cast gold or cast gold/electroforming; 3. determine retentive force kinetic characteristic depending on technology and material used to make conical double crowns;
3 Retention force assessment in conical crowns in different material combinations asses changes in retention force values depending on the number of in-and-out cycles corresponding to insertion and removal of dentures in different technological and material combinations. 2. Materials and methods The following sets of samples were prepared for testing the retentive force of conical double crowns: 1. Primary crown gold casting alloy, secondary crown gold casting alloy (Group 1). 2. Primary crown gold casting alloy, secondary crown made of pure gold by electroforming (Group 2). In both groups, sample sets were produced with the cone angles of 2, 4 and 6. For each set, 12 identical combinations were prepared, giving the total number of 72. All primary crowns were mounted on identical abutments made of non-precious Heranium Na alloy (Heraeus Kulzer, Hanau, Germany) and supplied with a cylindrical handle enabling their fastening. The shape of the crown part of the abutment was a copy of randomly chosen average lower canine, prepared with a moderate chamfer margin with average length of 6 mm measured from the margin of the preparation to the apex of abutment. The height of working walls of the abutment was 5 mm. In group 1, the primary crowns were made of precious alloy Aurix L60 (Safina, Jesenice, Czech Republic) by the casting method. The crowns were modelled using milling blue wax (Renfert, Hilzingen, Germany) to obtain a preliminary shape and were then milled on a Degussa F1 milling machine (GB Dental, Wesseling, Germany) with 2, 4 and 6 wax milling burs (Dr. Hopf, Langenhagen, Germany). After casting and preliminary processing of the casts, the axial walls were milled with 2, 4 and 6 metal milling burs (Dr. Hopf). The secondary crowns were modelled on the primary crowns together with handles shaped as those on the abutments. Then, they were cast from the same alloy as the primary crowns, cleaned from investment remains and potential artefacts from the casting process and fitted onto primary crowns. In group 2, the primary crowns were manufactured as in group 1, whereas the secondary crowns were prepared by electroforming. The primary crowns were coated with approximately 12 μm layer of electroconductive varnish Preciano Silberleitlack TK (Heraeus Kulzer, Germany). Next, they were placed in a galvanizer Combilabor CL-GF (Heraeus Kulzer) and poured with gold sulphate solution Precjano Gold (Heraeus Kulzer). During the electroplating cycle of 9-hour duration, a 0.3 mm thin layer of gold was created, forming a coping of the secondary crown on the primary one. Afterwards, the copings were placed in a liquid dissolving metallic varnishes. The electroplated copings so produced were cemented into handle moulders using Nimetic-cem cement (3M Espe, Seefeld, Germany). Photographs of the two sets of crowns prepared for testing are shown in Figs. 1a and 1b. Fig. 1a. Sample of primary cast crown and secondary electroformed coping prepared for testing Fig. 1b. Sample of primary and secondary cast crowns prepared for testing During the experiment joining separating cycles of the testing samples were carried out at a loading force of 75 N. The value of the loading force was chosen based on the work of Ohkawa et al. , who revealed that the retentive force in the double crowns increases with a rise in the loading force, but only to 50 N. Above this level, the retentive force does not practically depend on the loading force applied previously. Since during testing the loading force may show slight fluctuations, the accepted value of 75 N is expected to ensure steady test conditions. The duration of a single cycle, i.e., between successive loadings, was 1.8 s. An example of cyclic loading of a testing sample and retention force measurement is presented in Fig. 2. The loading curve shape approximates positive half of a sine curve, i.e., corresponds to mastication pattern .
4 38 J.K. PIETRUSKI et al. For the purpose of planned experiment a tribometer used for testing the properties of enamel and dental materials was modified . It operates through the pneumatic system for the loading of double crowns samples tested and provides computer control of load unload cycle parameters. Pneumatic driven beam makes downward and upward movements, which corresponds to denture insertion and removal. All parameters of the load cycle as well as gauges readings were transmitted to the computer where data was collected. Also, owing to special computer programme invented in Faculty of Mechanical Engineering, Białystok Technical University, basic parameters of the cycle, i.e., load amplitude, duration, intervals between successive loading cycles, were defined. Intervals between cycles were set for 1.8 s. The possibility of performing subsequent loading cycles without separating the primary crown and coping is an essential feature of this device and corresponds to denture loading during mastication. Therefore, it was possible to implement such a test protocol in which subsequent joining and separating of the connection were divided with a definite number of load cycles (masticatory events) without separation. This may be particularly important as nominally immobile connections used, e.g., in technical devices, show micro movements when being loaded, promoting the so called fretting, i.e., a destructive process within the area of the contacting surfaces . Test was performed with all the samples submerged in artificial saliva flow prepared according to Fusayama et al. s instructions . The thermostatic system allowed the temperature to be maintained at a steady level approaching that of the human body. Except for the thermostatic regulation, constant flow of liquid also ensured systematic removal of wear products off the friction area. For statistical analysis, due to certain data diversity, the Kruskal Wallis test of significance was used. Differences were considered statistically significant at p < The course of retention force changes obtained during laboratory test was smoothed out by trend line with the use of running mean with a step of 200. For this purpose Excel software (Microsoft Office, Seattle, USA) was used. For estimation of retention force changeability, special parameter called running standard deviation was elaborated. This parameter by analogy to running mean was calculated as standard deviation from consecutive 200 measurements of the retention force. For graphic comparison of data obtained this way for each group median, maximum, minimum and quartile 25 75% were calculated. 3. Results As the measurement data stored in the computer contain complete courses of the forces recorded by strain gauges and refer both to the loading and unloading forces (as shown in Fig. 2), at the beginning only retentive force values were selected from each course. To do this, a special procedure was developed in Excel calculation sheet that would allow identification of the minimum for each single cycle corresponding to the retentive force value. The results showing the retentive force kinetics averaged from 12 measurements for each study variant are presented in Figs. 3a, 3b and 3c. Fig. 2. Sample loading pattern: C single-cycle time; F maximum loading force; R retention force (A secondary crown, B primary crown) The graphs presented in Figs. 3 demonstrate significant differentiation in the level of retentive force depending on the cone angle of crowns which can be observed in the groups tested. The higher the angle value, the lower the average of the retentive force. However, the retention decrease was greater when the secondary crowns were cast from precious alloy (group 1), as compared to those produced by electroforming (group 2). With the cone angle of 2, the mean value of the retentive force in both experimental groups showed slight fluctuations, except for a certain variation in the kinetics of changes between the groups in the initial phase. The crowns of 4 and 6 taper showed a tendency toward a smaller or greater decrease in the average retentive force throughout the experiment.
5 Retention force assessment in conical crowns in different material combinations 39 force values for different material combinations. Comparing dispersion values in both groups, they are much lower (20 N) in group 1 as compared to group 2 (40 N). In order to show retentive force stability differentiation between the respective variants, standard deviation values were calculated for every successive 200 cycles (by analogy to the running average running deviation), and then graphs were drawn presenting the relationship between the number of cycles and standard deviation (Figs. 5a, 5b, 5c). Fig. 3a. Kinetics of the retention force for cone angle 2 (running averages) Fig. 4a. Retentive force values measured for chosen single 2 cone angle samples in group 2 Fig. 3b. Kinetics of the retention force for cone angle 4 (running averages) Fig. 4b. Retentive force values measured for chosen single 2 cone angle samples in group 1 Fig. 3c. Kinetics of the retention force for cone angle 6 (running averages) The findings obtained for single measurements indicate wide dispersions of retentive force values, which at first glance do not depend on the study variant. Figures 4a and 4b present example courses of changes in the retentive force. However, as opposed to Figs. 3, they show all the recorded values and not a trend line (running average). The graphs demonstrate a diversified character of dispersion of retentive Analyzing Figs. 5 it can be assumed that in group 1 with the cone angle 2 values of standard deviation show big variability with the dependence of cycles performed. In the beginning of the test values are about 5 N and decrease to about 3 N. Such values remain stable between 1000 and 6000 cycles. After 6000 cycles values are somewhere between 3.5 and 5 N which is similar to those at the beginning. With the cone angle 4 in group 1 standard deviation values are from 2.7 to 3.8 N till 6000 cycles. After this number of cycles they became more stable and till the end of experiments remained at about 3 N. In group 2 with cone angle 4 standard deviation values are higher
6 40 J.K. PIETRUSKI et al. the experiment. These findings are more clearly visible in Fig. 6, where the parameter called running standard deviation shows retention force changeability. 4. Discussion Fig. 5a. Standard deviation (progressive) of retention force (measured for the average of retention forces from 3 repetitions) for 2 cone angle Fig. 5b. Standard deviation (progressive) of retention force (measured for the average of retention forces from 3 repetitions) for 4 cone angle Fig. 5c. Standard deviation (progressive) of retention force (measured for the average of retention forces from 3 repetitions) for 6 cone angle from 4 to 6 N. At the cone angle of about 6 there is a clear difference between groups 1 and 2. In group 1, till 2000 cycles values are about 3 N and later on stay on a stable level of 2 N, whereas in group 2 these values are even four times higher (5 to 8 N) throughout The data obtained in the current study confirm partly previous findings concerning, e.g., the effect of cone angle of the crown on retentive force value. It has been well documented that the retentive force decreases with increasing angle , , . This is not surprising and has a theoretical support . However, it appears that the strength of this correlation is determined by the type of the material pair (coping fabrication technique). In conditions of the current study, the observations revealed a substantially greater effect of the cone angle on the retentive force (more precisely, on its average value) of the copings cast from the precious alloy, as compared to the pure gold copings made by electroforming. This effect is difficult to explain without additional tests, since the adhesive relationships between the contacting surfaces (as the base for friction resistances during separation of the two denture components) are affected both by elastic properties of materials (Young s modulus) and the type of material used, especially parameters of its crystal lattice . Furthermore, it is worth noting that the oral environment and cyclic character of loading during mastication create favourable conditions for specific frictional interactions to arise. One of those frictional mechanisms is fretting, i.e., a specific type of wear induced under load and in the presence of repeated relative surface micromotion. Microscopic observations of worn orthodontic appliances showed that these oral conditions often create fretting wear . The precision of crown fabrication may also play a role, particularly in the method of electroforming. At the same time, although in most cases the average retentive force value was found to decrease with an increasing number of the loading unloading cycles, the decrease was considerably milder than that observed by other authors , . This seems to be due to the fact that the experiments conducted by the authors cited were performed under dry conditions. Lack of liquid environment that would function as a lubricant could affect the accelerated wear of the contacting surfaces. As demonstrated earlier, repeatability of retentive force is as essential for normal functioning of the dentures supported by double crowns as its average level. The significance of retentive force stability can
7 Retention force assessment in conical crowns in different material combinations 41 be even greater, since with a considerable scatter of its values, there is a significantly increasing probability that too great forces (denture impaction) or too small forces (retention too small to maintain the denture stabilisation) may appear. In this situation, according to Weigl and Lauer , the material connections characterized by a lower, yet stable value of retentive force are more favourable than the ones having higher but less stable average retention. Accurate assessment of stability (repeatability) of retentive force is another problem. On the grounds of significantly varied pattern of changes, it seems that the proposed quantity of the so called running standard deviation reflects relatively well the character of these changes. Owing to such an approach, not only differences in stability between different test variants could be demonstrated but also the fact that retentive force stability may for certain connections change significantly during the experiment (e.g., for electroplated copings with 6 angle Fig. 5c). To determine the significance of differences in the stability of retentive force between different study variants, this value can be subjected to statistical analysis. Fig. 6. Box-and-whisker plot for progressive standard deviation: min-max, 25% 75%, median, respectively As shown in Fig. 6, the samples tested have a varied retentive force. The relatively high variability of the force observed for the crowns produced by electroplating seems a bit surprising. We are dealing here not only with considerable instability (high median value) but also with its changeable character during experiments (high quartile interval of 25% 75%). Weigl and Lauer reported that retentive force values were very stable in samples in which the primary crowns were made of zirconia ceramics whereas secondary crowns were made by elekctroplating . The explanation of this effect suggested by the authors, relating retentive force stability with precision fit ( made-to-measure ) of the secondary crowns should be considered reliable as well as lack of wedging effect when outer crown is electroformed and no gap is left between occlusal surfaces of crowns. Greater scatter of retentive force values for the electroplated crowns in group 2 (primarily casted) can be due to smaller precision fit associated with casting process itself as compared to casted alloy milled with burs and polished afterwards. The optimum parameters for retentive force stability were achieved for the samples with 6 cone angle formed by casting. This fact is difficult to interpret, particularly in the context of smaller precision associated with this technology. It seems that also other processes, apart from the adhesive effect, e.g., elastic deformation of the secondary crown, formation of vacuum during crowns separation, rheological properties of artificial saliva or capillary effect may also play a role in this case , . On the other hand, the samples with 6 cone angle formed by casting demonstrate the lowest values of retentive force, which seems to be too low for obtaining adequate retention of denture. For obvious reasons, the current study cannot explain all aspects associated with ensuring proper retention in conical double crowns. However, the apparatus designed and the methods suggested offer new possibilities in this field. Although the mean retention force value was found to be significantly influenced by geometry (cone angle) of the crowns, which confirms the findings reported in literature, the weight of this effect depends also on the materials used for crown making and technology applied , , . The so called running standard deviation parameter, proposed here, is an effective measure of retentive force stability, allowing not only the assessment of the stability level but also detecting any changes throughout the experiment. It should be emphasized that such a procedure can be applied only with the use of a device allowing current recording of retentive force values. 5. Conclusions In conclusion, within the limitations of current study it can be assumed that: the higher the angle value, the lower the average of the retentive force, dispersion of retention values is similar in material combination casting alloy/electroforming as compared to casting alloy/casting alloy,
8 42 J.K. PIETRUSKI et al. the conical crown made by the casting method from the precious alloy is better option of both tested in view of its high stability but only with cone angle 6. When cone angle is 2 or 4 (which is more often used in practice), stability of retention force with the passage of time is higher in combinations with electroformed outer crowns as compared to casted ones. These conclusions, however, have to be treated with caution as due to relatively considerable dispersion in the results, broader statistical material is needed to formulate ultimate proposals. Acknowledgements The authors are very grateful to DT Marek Janota (Dental Studio, ul. Agawy 34, Bielsko-Biala, Poland) for his help in preparation of samples used in the present study. References  MENSOR M.C., Attachment fixation for overdentures, Part I, J. Prosthet. Dent., 1977, 37,  MENSOR M.C., Attachment fixation for overdentures, Part II, J. Prosthet. Dent., 1977, 39,  BESIMO C., GRABER G.A., A new concept of overdentures with telescope crowns on osseointegrated implants, Int. J. Periodontics Restorative Dent., 1994, 14,  MINAGI S., NOBUKUNI N., NISHIGAWA G., SATO G., New telescopic crown design for removable partial dentures, J. Prosthet. Dent., 1999, 81,  WENZ H.J., LEHMANN K.M., A telescopic crown concept for the restoration of the partially edentulous arch: the Marburg double crown system, Int. J. Prosthodont., 1998, 11,  AKAGAWA Y., SEO T., OHKAWA S., TSURU H., A new telescopic crown system using a soldered horizontal pin for removable partial dentures, J. Prosthet. Dent., 1993, 69,  GREVEN B., LUEPKE M., VON DORSCHE H., Telescoping implant prosthesis with intraoral luted galvano mesostructures to improve passive fit, J. Prosthet. Dent., 2007, 98,  WEIGL P., LAUER H.-C., Advanced biomaterials used for a new telescopic retainer for removable dentures: ceramic vs. electroplated gold copings: Part I. Tribology effects, J. Biomed. Mater. Res., (Appl. Biomater.), 2000, 53,  PIETRUSKI J.K., PIETRUSKA M.D., SAJEWICZ E., A long term follow-up study of conical crown-retained dentures made with different technologies, Int. J. Periodontics Restorative Dent., 2012, 23,  STANČIĆ I., JELENKOVIĆ A., Retention of telescopic denture in elderly patients with maximum partially edentulous arch, Gerodontology, 2008, 25,  GÜNGÖR M.A., ARTUNÇ C., SONUGELEN M., Parameters affecting retentive force of conus crowns, J. Oral Rehabil., 2004, 31,  CHLADEK G., Durability evaluation of a friction couple intended for implantological stabilization of complete dentures, Acta Bioeng. Biomech., 2008, 10,  OHKAWA S., OKANE H., NAGASAWA T., TSURU H., Changes in retention of various telescope crown assemblies over longterm use, J. Prosthet. Dent., 1990, 64,  BAYER S., KEILIG L., KRAUS D., GRÜNER M., STARK H., MUES S., ENKLING N., Influence of the lubricant and the alloy on the wear behaviour of attachments, Gerodontology, 2010, doi: /j x  NEIL D.J., KYDD W.L., NAIRN R.I., WILSON J., Functional loading of the dentition during mastication, J. Prosthet. Dent., 1989, 62,  SAJEWICZ E., KULESZA Z., A new tribometer for friction and wear studies of dental materials and hard tooth tissues, Tribol. Int., 2007, 40,  STACHOWIAK G.W., BATCHELOR A.W., Engineering tribology, 3rd ed., Oxford: Elsevier Butterworth-Heinemann, 2005,  FUSAYAMA T., KATAYORI T., NOMOTO S., Corrosion of gold and amalgam placed in contact with each other, J. Dent. Res., 1963, 42,  STAMENKOVIĆ D., STANČIĆ I., Retention of removable partial denture with double crowns, Serbian Dental J., 2004, 51,  BUCKLEY D.H., Surface effects in adhesion, friction, wear, and lubrication, Tribology series 5, Elsevier Scientific Publishing Company,Amsterdam Oxford New York, 1981,  KLIMEK L., PALATYŃSKA-ULATOWSKA A., Scanning electron microscope appearances of fretting in the fixed orthodontic appliances, Acta Bioeng. Biomech., 2012, 14.
2 EDI Minimally invasive and patient-friendly treatment concepts using one-piece implants Renaissance of One-Piece Implants Hannes Thurm-Meyer, dentist, Bremen, Germany, Thomas Horn, master dental technician,
Implant Solutions for the Implant Patient: Diagnosis and Treatment Planning for Predictable Results David Little, DDS 6961 U.S. Highway 87 East San Antonio, TX 78263 Phone: (210)648-4411 Fax: (210) 648-6498
Restoration of a screw retained single tooth restoration in the upper jaw with Thommen Titanium base abutment. Dr. med. dent. David McFadden, Dallas County, USA Initial situation (single X-ray) Tooth 16
Utilizing Locator Attachments Step-by-Step Restorative Protocol Implant Bar Overdentures offer a removable implant solution for edentulous patients desiring a stable and esthetic prosthesis that improves
FABRICATING CUSTOM ABUTMENTS LUC AND PATRICK RUTTEN How much should a Dental Technician know about the clinical aspects of implantology? The answer is clear: as much as possible. This is the distinction
(Protocol A Includes Wax Setup) Step-by-Step Restorative Protocol A The BruxZir offers a fixed, all-zirconia implant solution for edentulous patients desiring a stable and esthetic replacement for removable
CHAPTER 8 PROSTHETIC TEETH DEFINITION PROSTHETIC TEETH are the artificial substitutes for the missing natural teeth. FUNCTIONS to: The functions of prosthetic teeth are 1. Restore the esthetic, phonetic
The concept Simplicity and versatility for prosthesis fixation The concept Experience the freedom in prosthesis fixation Simple and secure fixation of implant-supported prostheses is essential for successful
Abutment fracture in a bridge supported by natural teeth and implants Authors_Dr Gregory-George Zafiropoulos, Dr Giorgio Deli & Dr Rainer Valentin, Germany/Italy _Introduction Implant treatment has evolved
Case Reports in Dentistry Volume 2012, Article ID 264620, 4 pages doi:10.1155/2012/264620 Case Report Custom Metal Occlusal Surface for Acrylic Resin Denture Teeth to Enhance Wear Resistance: A Case Report
CDT 2015 Code Change Summary New codes effective 1/1/2015 Code Nomenclature Delta Dental Policy D0171 Re-Evaluation Post Operative Office Visit Not a Covered Benefit D0351 3D Photographic Image Not a Covered
PROSTHETIC PROCEDURE for HG IMPLANT SYSTEM PROSTHETIC PROCEDURE for HG IMPLANT SYSTEM HG Implant System Contents Cement retained restoration Rigid abutment When abutment reduction is unnecessary When abutment
11. The Effect of Abutment Tooth Connection with Extracoronal Attachment using the Three Dimensional Finite Element Method - Part 2. The Construction of Finite Element Model from CT Data - Ando A., Nakamura
CHAPTER 10 RESTS AND DEFINITIONS A REST is any rigid part of an RPD framework which contacts a properly prepared surface of a tooth. A REST PREPARATION or REST SEAT is any portion of a tooth or restoration
priti crown Your patients deserve you 3 and you deserve the priti crown So close to nature priti crown is a high-tech solution for making perfect crown and bridge restorations using state-of-the-art CAD/CAM
Accelerated Patient Rehabilitation Providing The Tools Necessary For An Immediate Solution: NanoTite Implants QuickBridge Provisional Components Navigator System For CT Guided Surgery Initial Patient Presentation
SCD Case Study Treatment Considerations for Implant Rehabilitation Multiple surgical and restorative factors play a role in the treatment planning of implant restorations for the edentulous patient (Ali
Implant Parts A Radford Heath Guide http://www.radfordheath.com 1 Disclaimer The information given in this document has been provided in good faith for basic information purposes only and the information
PROSTHODONTICS RESTORATIONS - INLAY AND ONLAY CROWNS BRIDGES VENEERS IMPLANTS RESTORATIONS Due to improved dental hygiene and the use of fluoride, there is a reduction in tooth decay found in our patients.
USAGE OF SELECTIVE LASER MELTING TECHNOLOGY CAPABILITIES IMPLEMENTATION FOR TEETH IMPLANTS METAL CONSTRUCTION IN TU-SOFIA George TODOROV, Nikolay NIKOLOV, Victor MITOV, Yavor SOFRONOV Technical University
Introduction of Removable Partial Denture By : Dr Zaihan Ariffin BDS(Malaya), Grad. Dip In Clinical Dentistry (Adelaide), Doctor of Clinical Dentistry (Adelaide), FRACDS (Australia) Aims & Objectives What
ATLANTIS ISUS the benchmark for CAD/CAM suprastructures For all major implant systems Patient satisfaction meets clinical benefits ATLANTIS delivers leading CAD/CAM patient-specific restorative solutions
Replacement of the upper left central incisor with a Straumann Bone Level Implant and a Straumann Customized Ceramic Abutment by Dr. Ronald Jung and Master Dental Technician Xavier Zahno Initial situation
IMPLANT DENTISTRY EXAM BANK 1. Define osseointegration. (4 points, 1/4 2. What are the critical components of an acceptable clinical trial? (10 points) 3. Compare the masticatory performance of individuals
Crown and bridge Lecture.1 Dr.hasan AL Rrammahi The dental specialty concerned with the making of artificial replacements for missing parts of the mouth and jaw. Also prosthetic dentistry or prosthodontia.
Lecture.1 Dr.Adel F.Ibraheem Crown and Bridge: It s a branch of dental science that deals with restoration of damaged teeth with artificial crown replacing the missing natural teeth by a cast prosthesis
www.jird.com CLINICAL PERSPECTIVES Inside this issue: Using digital technologies to address aesthetic challenges in the anterior maxillae A Publication 2011 No. 1 3 JIRD Article Title (continued) aesthetic
1/2 point CDT documented scientific credit. See Page 41. Implants in your Laboratory: Abutment Design By Leon Hermanides, CDT A patient s anatomical limitations have the greatest predictive value for successful
Another Implant Option for Missing Teeth with Challenging Symmetry Patrick Gannon, DDS and Luke Kahng, CDT Introduction A 58 year old male had been missing teeth #7=12 for approximately 28 years. During
Dental Implants - the tooth replacement solution Are missing teeth causing you to miss out on life? Missing teeth and loose dentures make too many people sit on the sidelines and let life pass them by.
CAD/CAM technology supporting successful implant therapy Suheil M. Boutros, DDS, MS, Manuel Fricke, DT Modern implantology opens up new treatment options for individuals with only minimal or no remaining
A stable yet removable prosthesis for edentulous patients A little friction is a good thing ATLANTIS Conus concept Redefining stability and comfort The ATLANTIS Conus concept a conometric solution A conometric
EXPERIENCE USA RUSSIA GREECE OFFERING EXCITING DIGITAL OPPORTUNITIES AROUND THE GLOBE ROMANIA FEB. 2016 DIGITAL DIGITAL DENTISTRY Technology is Changing Dentistry Dentistry is evolving, starting from diagnosis
The WeldOne concept Facilitating stable and durable chairside solutions Courtesy Dr. Marco Degidi, Bologna, Italy With the help of WeldOne Welding Unit and special welding components, a titanium wire is
Straumann Dental implant system ONE SYSTEM ONE INSTRUMENT KIT VARIOUS TREATMENTS For various treatments* The Straumann Dental Implant System offers you and your patients efficient and esthetic implant-borne
BICON DENTAL IMPLANTS The Bicon Dental Implant System, since 1985, has offered discerning dentists the ability to provide secure implant restorations that look, feel, and function like natural teeth. With
E F F I C I E N C Y T H R O U G H S I M P L I C I T Y February 2012 The AP Prettau Bridge By Jörg Müller, MDT Developing a plan, turning it into a protocol and then following every step precisely, will
Implant Restorative Guide: Patient Edition We are most fortunate at Precision Dental Arts to be working with some of the best doctors across the country. With over 30 years of experience restoring dental
Managing Wear and Esthetics KEY Occlusal Dental Components: - Centric contacts - End-to-end contacts - Pathways KEY: In order to increase the predictability in managing patients with wear, it is advisable
Against All Odds A No Bone Solution Long-term success of osseointegrated implants depends on the length of the implants used and the quality and quantity of bone surrounding these implants. As surgical
Electronic Health Records in Continuous Shared Dental Care Taťjana Dostálová 1, Jana Zvárová 2, Zuzana Teuberová 1, Michaela Seydlová 1, Martin Pieš 2, Josef Špidlen 2 1 Department of Prosthodontics, First
Taking the Mystique out of Implant Dentistry Dr. Michael Weinberg B.Sc., DDS, FICOI What is Restorative Implant Dentistry? Restorative implant dentistry involves taking a few simple mechanical principles
Prosthetic treatment planning on the basis of scientific evidence. Pjetursson BE, Lang NP. J Oral Rehabil. 2008 Jan;35 Suppl 1:72-9. Faculty of Odontology, University of Iceland, Reykjavik, Iceland, and
Final (20101018) The College of Dental Surgeons of Hong Kong Guidelines for the Provision of Dental Implants 1. Introduction Restorations supported by dental implants have become an accepted method for
Full Crown Module Restoration / Tooth # Full Gold Crown (FGC) / 30 Extensions: Porcelain Fused to Metal (PFM) / 12 All Ceramic / 8 Learner Level 1 Mastery of Tooth Preparation Estimated Set Up Time: 30
Review Article The total occlusal convergence of the abutment of a partial fixed dental prosthesis: A definition and a clinical technique for its assessment John S. Mamoun 1 Correspondence: Dr. John S.
STEP-BY-STEP INSTRUCTIONS ON THE PROSTHETIC PROCEDURES Straumann Anatomic IPS e.max Abutment The ITI (International Team for Implantology) is academic partner of Institut Straumann in the areas of research
CDT 2016 Current Dental Terminology American Dental Association procedure codes (CDT codes) are the recognized dental codes set by the Federal Government. CDT codes are used for dental claim transactions
PATIENT INFORM CONSENT for IMPLANT RESTORATION Rev 04.2012 Implant placement and restoration involves two major stages: surgical placement of the implant(s) followed by the restoration of the implant after
Screws Screws for definitive use. Made from medical grade 5 ELI Titanium Integrity and soundness guaranteed by stress tests of up to 150% of their nominal torques. Their designs ensure a perfect fit with
Step-by-Step Virtual Implant Planning MIS Corporation. All Rights Reserved. MIS Warranty: MIS exercises great care and effort in maintaining the superior quality of its products. All MIS products are guaranteed
Smile Confidently With DIEM 2 Immediate Full Arch Rehabilitation Immediate Full Arch Rehabilitation * Edentulism and failing dentition continue to be major health challenges affecting millions of people
LEBENSLAUF Dent. Dr. ÖZGE ÖZTÜRK 1. EDUCATION AND TRAINING Year Position/Title School/University Field 1987-1994 Student T.E.D. Ankara College, Ankara, TURKEY High School (honour student) 1994-1999 Student
BIOMECHANICAL ANALYSIS OF NORMAL AND IMPLANTED TOOTH USING BITING FORCE MEASUREMENT B K Biswas 1 S Bag 2 & S Pal 3 1. Dept. of Dental Surgery, Associate Professor, KPC Medical College & Hospital, Kolkata,
For all major implant systems A removable prosthesis with the comfort of a fixed restoration ATLANTIS Conus concept ATLANTIS Conus concept offers several advantages for the patients: A stable but removable
A Review of Implant Abutments - Abutment Classification to Aid Prosthetic Selection Sanjay Karunagaran, B.D.S., D.D.S., M.S.D., Gregory J. Paprocki, D.D.S., Russell Wicks, D.D.S., M.S., Sony Markose, B.D.S.,
Direct Fillings: Amalgam Dental amalgam is a stable alloy made by combining mercury, silver, tin, copper and sometimes other metallic elements. Amalgam fillings can be placed in one appointment. Why you
Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,
Basic information on the Straumann Variobase Abutment. 1 Straumann is the industrial partner of the ITI (International Team for Implantology) in the areas of research, development, and education. Contents.
The Transition from Teeth to Implants and the Use of Post-ceramic Soldering Basil Mizrahi, BDS, MSc, MEd* Anthony Laurie, RDT, FCGI, FBIDST** D ental implants have become a widely accepted and successful
Improving Esthetics with Sequential Treatment Planning and Implant-Retained Dentures by Timothy F. Kosinski, DDS, MAGD While oral function is the primary concern for most patients, the importance of esthetics
(19) TEPZZ 69 _ZA T (11) EP 2 692 3 A2 (12) EUROPEAN PATENT APPLICATION published in accordance with Art. 13(4) EPC (43) Date of publication: 0.02.14 Bulletin 14/06 (21) Application number: 1276632.0 (22)
procedures & products NOBELESTHETICS including Procera First from Nobel Biocare. NOBELPERFECT, (NP, RP, WP), NOBELDIRECT (NP, RP, WP), Brånemark System, NOBELREPLACE and NOBELSPEEDY Implants. A complete
TRI Product NewsFlash December 2015 Study Overview 2015 Dear Partners Year in, year out, we are screening all major scientific journals to ensure that our TRI Performance Concept still reflects the latest
Press Abutment Solutions Efficiency and esthetics redefined all ceramic all you need More press ceramic options... Press ceramics have been synonymous with the ideal combination of accuracy of fit, shape
1 Presenter: Dr. Sana Ehsen Supervisors: Dr. Farhan Raza Khan 2 A dental implant (also known as an endosseous implant or fixture) is a surgical component that interfaces with the bone of the jaw to support
* This is in addition to the embedded Preventive Plan (see procedure list at deltadentalco.com/kp_preventive. BASIC SERVICES Minor Restorative Services D2140 Amalgam 1 surface, primary or permanent D2150
Discovering the Benefits of Dental Implants A Patient s Guide Are You a Candidate for Dental Implants? How you feel about yourself affects your relationships, your confidence, and your overall well-being.
Dental implant impression transfer components Dr Koray Feran and Anthony Spencer look at the properties, materials and laboratory impression procedures Dental implant impression transfer components (also
Number 3 $1.25 The Most Frequently Asked Questions About Dental Implants... A Consumer s Guide to Understanding Implant Treatment If you are like most people considering dental implants, you probably have
Procera Alumina vs. Feldspathic Porcelain How to Achieve Shade Harmony With Different Restorations Luke S. Kahng, CDT Key Words: Stump shade, Feldspathic Porcelain, Zirconia, Alumina, LSK Treatment Plan
Saudi Fellowship In Dental Implant (SF-DI) Prepared and Updated by Dr. Arwa AL-Sayed Consultant Periodontics and Dental Implants M E M B E R S Dr. Arwa AL-Sayed Dr. Abdulhadi Abanmy Dr. Ali AL-Ghamdi Dr.
PAGE 1 of 5 References Related ACA Standards 4 th Edition Standards for Adult Correctional Institutions 4-4369, 4-4375 PURPOSE To provide guidelines for determining appropriate levels of care and types
Full Mouth Restoration with Screw-Retained Zirconia Bridges A DENTIST-LAB RELATIONSHIP THAT WORKS Dentist: Steven P. Stern, DMD Windsor Dental Center New Windsor, NY Dental Laboratory: InnoDDS Dental Laboratory
Cerobear Spindle Bearings for Machine Tool Applications Cerobear Spindle Bearings About CEROBEAR Committed to the abbreviation CEramic in ROlling BEARings, CEROBEAR GmbH is the renowned world leader in
September 13-16, 2009 Waikoloa, HI September 13-16, 2009, Waokoloa, Waikoloa, HI Biomimetic i Tooth Implants by Electron Beam Melting Mari Koike, DDS, PhD 1 ; Gilbert Chahine 2 ; Radovan Kovacevic, PhD
Your consent to our cookies if you continue to use this website.